Investigation of Activation Process of Membrane Electrode Assembly Obtained By Various Formulation Conditions for High-Temperature Polymer Electrolyte Fuel Cell
Authors: Kim Do Hyung , Lee Eun Ae , Pak Chanho 
Published: February 2020

Recently, the polymer electrolyte membrane fuel cells (PEMFCs) have attracted the great attention as energy conversion devices for powertrain for the fuel cell electric vehicle and a residential combined heat and power system due to the zero-emission of harmful gas and high energy efficiency. To overcome of the drawbacks of perfluorosulfonic acid (PFSA) membrane and Pt poisoning by CO, the high-temperature PEMFC (HT-PEMFC) has been developing over decades, which has significant advantages as compared to low-temperature PEMFC (LT-PEMFC). For example, it has a much better fuel tolerance, enhanced the reaction kinetics and a simple water management [1,2]. However, the practical power density of membrane electrode assembly (MEA) for HT-PEMFC is much lower than that of LT-PEMFC because of the huge activation loss by acid poisoning [3–5]. Thus, a large amount of Pt is required in the electrode to ensure the sufficient power and long-term durability, which is a critical issue for HT-PEMFC. Therefore, one of the most critical issue for the HT-PEMFC is the decreasing the Pt amount in the electrode without sacrificing the MEA performance [5]. In addition, the fabrication of electrode using the advanced supported catalyst is the very important topic for revealing the improved catalytic activity into performance of MEA [2,5].

In this study, various formulation parameters for making the catalyst slurry using ball-milling were investigated to obtain the smooth electrode for MEA. The parameters are the presence of a viscosity agent, the solid content, and the amount of binder for the MEA of HT-PEMFC. When the viscosity agent is added in the 2.5 wt.% in the catalyst slurry, the slurry is very suitable for making a coated electrode on the gas diffusion layer (GDL). On the contrary, while when the amount of viscosity agent is increased over than 5 wt.%, the electrode is not completely dried. The optimum solid content of catalyst in the slurry was determined in the range of 12 wt.% because if the amount of catalyst exceeded the 14wt.%, the electrode is peeled off severely after drying. The open circuit voltage and performance of MEA under HT-PEMFC condition is depended significantly on the amount of polyvinylidene fluoride (PVDF) in the catalyst slurry. The voltage at a very small current density at 0.008A/cm2 of MEAs with different amount of PVDF was decreased from 0.775 to 0.735 V by increasing the 10wt.% to 30 wt.% of PVDF, which provide the increase of the activation overpotential by poisoning of phosphoric acid on the Pt catalyst. However, the performance of MEA at 0.6A/cm2 was maximized as 0.44 V at the 30wt.% of PVDF in the catalyst slurry, which suggests that the Ohmic overpotential decreased with increasing the PVDF amount. In summary, for maximizing the MEA performance under HT-PEMFC at 150℃, the various conditions for the manufulation of electrode was invesitgated. The amount of PVDF has a significant effect on the performance of MEA.

[1] J. Zhang, Y. Xiang, S. Lu, and S. P. Jiang, Adv. Sustainable Syst.
2, 1700184 (2018).

[2] D. J. You, D. H. Kim, J. R. De Liled, C. Li, S. G Lee, J. M. Kim, and C. Pak, Appl. Catal. A: General
562, 250–257 (2018).

[3] R. E. Rosli, A. B. Sulong, W. R. W. Daud, M. A. Zulkifley, T. Husaini, M. I. Rosli, E. H. Majlan, and M. A. Haque, Int. J. Hydrogen Energy
42, 9293–9314 (2017).

[4] A. Chandan, M. Hattenberger, A. El-kharouf, S. Du, A. Dhir, V. Self, B. G. Pollet, A. Ingram, and W. Bujalski, J. Power Sources
231, 264–278 (2013).

[5] S.-W. Choi, J. O. Park, C. Pak, K.H. Choi, J.-C. Lee, and H. Chang, Polymers
5, 77–111 (2013).